Thermally Activated Delayed Fluorescence as an Emerging Trend in Optoelectronics
The transformation of electrical energy into visible light has remained an important issue for scientists and engineers, even more than a century after the development of the incandescent lightbulb by Swan, Edison, and others.1,2 One of the new emerging topics in this niche of material sciences is emitting materials that feature thermally activated delayed fluorescence (TADF). Although TADF has been known since 1960,3 the potential use of TADF emitters in optoelectronic devices has been proposed independently by several groups led by Adachi et al.45.–6 (organic and tin emitters), Deaton et al.,7 Yersin et al.,8 and others.910.11.–12 The rise of the TADF-topic is reflected by an exploding number of new peer-reviewed publications dealing with it in general (Fig. 1), peaking close to 200 in 2015. Note that Refs. 4–8, which propose and show the use of such materials in organic light-emitting diodes (OLEDs) for the first time, have been published between 2009 and 2012, suggesting that the rise of this concept was directly related to a potential (industrial) application in OLEDs. Occasionally, synonyms such as “singlet harvesting”1314.15.–16 or “E-type fluorescence”7,17,18 are also being used in the literature.
The aim of this review article is to briefly introduce this concept and outline its impact on photonics, especially with respect to its potential concerning the realization of energy-efficient solid-state lighting and display devices. The scope of this article does not include any in-depth discussion of the molecular structure of TADF molecules or device architectures, which can be found elsewhere.1920.21.–22
What Is Thermally Activated Delayed Fluorescence?
Upon recombination of charge carriers in any electroluminescent device, two different types of excitons are formed: singlet excitons having a spin and triplet excitons with .23 Due to quantum statistics, the relative probability for the formation of singlet and triplet excitons is 25% to 75%.13,24,25 In order to realize efficient OLEDs, it is crucial to harvest both singlet and triplet excitons for the generation of photons. Currently, there are three main emissive mechanisms available to harvest excitons: fluorescence, phosphorescence as well as TADF. A schematic overview of these mechanisms is shown in Fig. 2.
On a side note, there are also more complex schemes, which usually require at least a bimolecular, often trimolecular emitting mechanism (e.g., multiple species between which energy can be transferred) such as -type delayed fluorescence or triplet–triplet annihilation,2627.28.–29 hyperfluorescence,30 exciplex emission,6 and exciplex-assisted emission.3132.33.–34 These mechanisms will not be covered in this article.
Fluorescent molecules have a relatively large energetic difference between the and state. This difference is also known as the singlet–triplet splitting or ().13 In addition, they usually show very weak intersystem crossing (ISC) and reverse intersystem crossing (rISC), meaning that the transformation of singlet () into triplet excitons () and vice versa is quantum-mechanically forbidden, therefore both slow and unlikely.23 The same is true for any transitions between and the singlet ground state .35,36 Because of these limitations, triplet excitons cannot be harvested with fluorescence, limiting the overall efficiency of such OLEDs to 25%.13 An archetypical fluorescent OLED emitter is aluminum-tris-(8-hydroxyquinoline) (; Fig. 3).3738.39.–40
Phosphorescent molecules41 share a rather larger () value with their fluorescent counterparts. On the other hand, ISC is very strong, leading to a prompt transformation of any singlet into triplet excitons. Because of the ISC, which is the result of the presence of heavy transition metals such as iridium, platinum, and osmium, the transition between and is possible.35,36 Connected to this is the term triplet harvesting, because all excitons are harvested via the triplet state .13 With this, it was first possible to harvest all generated excitons, which resulted in highly efficient OLEDs.42,43 An archetypical phosphorescent OLED emitter is iridium-tris-(2-phenylpyridine) (; Fig. 3).44–45
TADF molecules have a low (), typically in the order of several hundreds of meV, and mediocre ISC and rISC.21 Although direct transitions between and are still forbidden, it is possible to go from back to by means of rISC, if the thermal energy is sufficient. Compared with normal fluorescence, where the excited-state lifetime is in the order of ns, the excited-state lifetime is longer, often in the order of or more—the term TADF accounts for these observations. Occasionally, the term singlet harvesting1415.–16,46 is used, because all excitons are harvested via the singlet state .13 A typical TADF emitter is tetrakis--carbazoyl-isophthalonitrile (4CzIPN; Fig. 3).5,4748.–49
In summary, TADF is an alternate concept, which can help to realize efficient OLEDs with maximum efficiency. It competes with phosphorescence, the commercial state-of-the-art solution for efficient OLEDs.
Conceptual Background of Thermally Activated Delayed Fluorescence
Molecular Design Principles
Without going too much into detail, all TADF emitters consist of donor and acceptor moieties. In a way, they are similar to so-called ambipolar host molecules and often even contain similar building blocks, which are either arranged in a different way or used in different combinations in order to realize the large bandgap, which is needed to accommodate dopant molecules.5051.52.53.54.–55 In both hosts and TADF emitters, donor moieties are electron-rich functional units that have a rather deep HOMO, which allow them to be oxidized easily and partake in the transport of holes. Contrarily, acceptor moieties are electron-deficient functional units with a deep LUMO. They can be reduced and thus partake in the transport of electrons. Figure 4 contains the molecular structure of various donor units, while acceptor units are shown in Fig. 5.
It is apparent that—as of today—there is much more variation found on the acceptor part than on the donor part of TADF emitters.19 As indicated in Fig. 4, the vast majority of all published organic TADF emitters contain substituted carbazole-5657.58.–59 or arylamine-type donors.6061.–62 In most cases, the connection to the acceptors is realized via the aromatic nitrogen. On the acceptor-side (Fig. 5), one can find a plethora of nitrogen-containing heterocycles,63,64 as well as various benzonitriles.4748.–49,56,57,59,65,66 A third acceptor-class is sulfones,31,54,58,60,67,68 which seems to be particularly useful to realize deep-blue TADF emission.
The color of the TADF emitter depends on the choice of the donor and acceptor moieties. Approximately, the choice of the donor dictates the HOMO, while the acceptor dictates the LUMO. The energetic difference between HOMO and LUMO is the bandgap, which is closely connected to the emission color of the emitter. Roughly, a bandgap of ca. 2.8 eV (450 nm) relates to blue emission, while 1.9 eV (650 nm) gives red emission.23 In Sec. 1, () was introduced as the most crucial parameter for TADF. This parameter is highly dependent of the localization of the Frontier orbitals HOMO and LUMO.69,70 The better the separation (or the smaller the overlap between HOMO and LUMO), the smaller (), which facilitates efficient ISC and rISC. From a design point of view, the overlap of HOMO and LUMO can be manipulated by the way in which the donor and acceptor moieties are connected. This is emphasized by analyzing the properties of different combinations of triphenyltriazine-type acceptors (Trz) with carbazole-type donors (Cz and mCz or ), which have been published by Lee et al.71,72 This work lead to the TADF emitters DCzTrz, TCzTrz, DCzmCzTrz, and TmCzTrz, which are shown in Fig. 6. Addition of an additional carbazole or dimethylcarbazole to DCzTrz changes the triplet energy () from 0.23 to 0.16 and 0.07 eV, respectively, in TCtTrz and DCzmCzTrz.
The photoluminescence quantum yield and excited-state lifetime are—in this case—connected to (): it changes from 43% at (DCzTrz) to 100% at (TCzTrz) and 99% at (DCzmCzTrz). Note that the color of the four emitters shown in Fig. 6 depends on the choice of the donor unit. The carbazole-emitters DCzTrz and TCzTrz show peak electroluminescence around 480 nm, while the emitters with dimethylcarbazole, , emit around 500 nm. This can be attributed to a variation of the HOMO energy of carbazole, which is slightly raised when electron-rich methyl groups are added.
When comparing ambipolar host molecules with TADF dopands, the differences are often subtle. Examples are pCzOXD,73 a fluorescent, ambipolar host molecule and 2PXZ-OXD,74 a TADF emitter, which are shown in Fig. 7. They both feature diphenyloxadiazole (OXD) as the acceptor unit (not shown in Fig. 5) as well two carbazole- (Cz) or phenoxazine-donors (PXZ) per molecule. Apart from the different HOMO energy, which leads to a smaller bandgap for 2PXZ-OXD due to the shallower HOMO of phenoxazine, the twist angle between the donor and the phenyl-substituent is different with a reported value based on DFT calculation of 52 deg for pCzOXD73 and 75 deg for 2PXZ-OXD.74 The larger twist breaks the conjugation between the donor and acceptor, which leads to a well-separated HOMO and LUMO and a small () for 2PXZ-OXD,74 while the HOMO is totally delocalized for 2PXZ-OXD, as suggested by DFT calculations.73
Organic Versus Copper Thermally Activated Delayed Fluorescence Organic Light-Emitting Diodes
In Sec. 2.1, we highlighted organic, small-molecule TADF emitters. For metal–organic TADF emitters, the same design principles are also essentially true (Fig. 8). In this case, the HOMO is often located on metal (or metal-halide) centered orbitals, while N-heterocyclic ligands (which are also being used in organic TADF emitters, refer to Fig. 5) house the LUMO. The same is also true for polymeric TADF emitters, where the HOMO and LUMO are located on different monomers of the polymer strand.75
Both organic66,78,79 and metal–organic TADF emitters77 have been shown to reach the maximum theoretical OLED efficiency, which is in the order of 20% to 25% external quantum efficiency in cases where no light-extraction technology is applied.13 For clarity, the molecular structures of metal–organic TADF emitters are not discussed here. This has already been covered elsewhere.8081.–82
Current Strengths and Weaknesses of Thermally Activated Delayed Fluorescence–Organic Light-Emitting Diode
In terms of efficiency, TADF is already directly competing with phosphorescent OLEDs,66,78,79 even though the first TADF OLED was published only 5 years ago.63 In terms of stability, there are some promising results.72,83 With 4CzIPN (see Fig. 2), values of over 10,000 h (starting luminance of ) have been reported. However, there still exists a gap that needs to be bridged prior to commercialization.
It has been pointed out that TADF emitters partake in the charge transport in the OLED architecture, which are currently used.83 This is a result of the high doping concentrations, ranging from 6% up to neat emitter films that are usually being employed, which facilitate charge transport, as well as the current lack of host and blocking materials with properly aligned energy levels and high-triplet energies.84,85 In another study, it was demonstrated that charge-carrier-induced formation of small (e.g., as a result of unimolecular processes) and large molecular weight (e.g., as a result of multimolecular processes) degradation products occurs, which suggests bond formation as well as bond cleavage needs to be prevented. This is a general problem for all organic semiconductors, but is generally solvable when reaching a certain level of maturity.86 The authors also pointed out that 3,3-Di(9H-carbazol-9-yl)biphenyl, a host that is often used with TADF emitters, is in fact not sufficiently stable upon UV irradiation.87 This further suggests that the development of hosts and supporting materials needs to be investigated in parallel to the actual material development.
A big issue is the excited-state lifetime or emission decay time of materials. Apart from efficiency roll-off,8889.–90 the loss of OLED efficiency at high currents, this is also likely to affect the operational stability. Unfortunately, no straightforward structure–property relation has yet been identified to systematically modify the excited-state lifetime of TADF emitters. Especially metal-free TADF emitters often suffer from long excited-state lifetimes up to the millisecond regime,65,90 while ideally, the excited-state lifetime is in the order of or even less.13 For the diphenylsulfone acceptor (see Fig. 5), excited-state lifetimes in the order of ms are achieved when donors such as tert-butyl-carbazole are used,68 while in a similar system with dimethoxycarbazole, only several are reported.91 This cannot be rationalized or predicted with the current level of understanding. At this point, no general design rules exist on how to specifically design TADF molecules with very low-excited-state lifetime.
Potential Economic Impact of Thermally Activated Delayed Fluorescence: Overcoming the Blue Gap
OLEDs have successfully been introduced in commercial products, such as tablet personal computers, smartwatches, and smartphones in the last few years, thanks to breakthroughs that led to the realization of stable devices with good efficiency. The first commercial successes should not distract from the fact that there is much room for improvement. Currently, the most pressing material issue in OLEDs is the bluegap (Fig. 9): In modern, commercial OLEDs, fluorescent materials92 are used in addition to phosphorescent materials, even though this leads to an increased power consumption. The main reason for this is the unavailability of stable deep-blue phosphorescent emitters.93
Similar to any other display technology, OLEDs display consists of red, green, and blue pixels. While red and green pixels rely on energy-efficient, phosphorescent materials, blue phosphorescent OLEDs never reached the necessary color purity and stability to allow for commercialization. It needs to be said that academic and industrial institutions tried to solve this issue with blue phosphorescent materials without success for the last 15 years,94126.96.36.199.99.–100 suggesting that much like the low efficiency of fluorescent OLED materials, the instability of blue phosphorescent materials might be an intrinsic property and that innovative material concepts are required to close the bluegap. This means that as of today, no efficient and stable blue OLED pixels are available. The consequences are drastic, because the human eye is relatively insensitive to blue light, which means that a fairly large amount of blue pixels is needed in any display.
The scope of this problem can be illustrated with a back-of-the-envelope calculation: typical OLED devices have displays with fluorescent blue emitter materials. Due to the aforementioned color sensitivity, 52% of the active display consists of blue pixels (Table 1). With a standard 2600-mAh-capacity battery, such a device plays up to 12.5 h of video.
Representative size of AMOLED pixels for smartphones.
|Average area in a display (μm2)||Relative area (%)|
|Sum||1050||Percentage of total active area|
Using a deep-blue TADF of phosphorescent emitter will allow for a reduction of the blue pixel area due to the greater light output. Assuming that the energy consumption of blue pixels is decreased by only 66% (corresponding to an efficiency increase by a factor of 3), the energy consumption of the whole display will be decreased by 33% and the battery lifetime of the video mode will be increased from 12.5 to more than 16 h. Note that the theoretical efficiency increase when using blue TADF or phosphorescence technology is even larger than assumed here (factor of 4 instead of 3!).
The first promising steps have already been made to put this into reality: in several cases, efficiency values of more than 20% have been demonstrated in deep-blue TADF OLEDs.64,68,71,72,101,102 The lifetime of blue TADF OLEDs is currently in the order of 50 h (, starting luminance ), which was achieved for derivatives of DDCzTrz (structure, see Fig. 6).72
Given that the issues that were outlined in Sec. 3 are adequately addressed, and TADF technology has the potential to close the bluegap.
Considering that first-world societies use up to 30% of their electric energy either for direct lighting or for the illumination of the displays of large-area TVs or portable devices, the development of stable and efficient deep-blue OLEDs is a problem with great economic relevance. It is evident that after many unsuccessful attempts to realize this with phosphorescent materials, new approaches such as TADF need to be investigated. Apart from aspects such as general chemical stability against dissociative and associative reactions, the focus of future work should be directed toward a more in-depth understanding of the parameters, which can be used to tune the excited-state lifetime. Without it, material development is highly dependent on empiric brute-force approaches and luck, which significantly reduces the probability of success.
In this review, the TADF concept was introduced. With a modular approach, TADF molecules can be designed from donor and acceptor units. Also, the current strengths, especially the very high device efficiency, as well as weaknesses such as the often long excited-state lifetime, have been addressed. The great economic potential of blue TADF technology was outlined, which is one of the main driving forces for future academic and industrial research in this field.
This work has been sponsored by the German Federal Ministry of Education and Research. BMBF in the funding programs “cyCESH” and “cyFLEX.” Also, we acknowledge funding from the European Union in the LEO Project (H2020-ICT-2014-1 call). D.V. thanks the R&D Division of CYNORA and his collaboration partners, among them Stefan Bräse, Clemens Heske, Uli Lemmer, and Christopher Barner-Kowollik (Karlsruhe Institute of Technology), Hartmut Yersin (University of Regensburg), and Franky So (North Carolina State University) for their continued support.
R. Friedel and P. Israel, Edison’s Electric Light: Biography of an Invention, Rutgers University Press, New Brunswick, New Jersey (1986).Google Scholar
W. H. Meadowcroft, Thomas Alva Edison, Harper Brothers Publishers, New York (1911).Google Scholar
C. A. Parker and C. G. Hatchard, “Triplet–singlet emission in fluid solutions. Phosphorescence of eosin,” Trans. Faraday Soc. 57, 1894 (1961).TFSOA40014-7672http://dx.doi.org/10.1039/tf9615701894Google Scholar
A. Endo et al., “Thermally activated delayed fluorescence from Sn4+-porphyrin complexes and their application to organic light emitting diodes—a novel mechanism for electroluminescence,” Adv. Mater. 21(47), 4802–4806 (2009).ADVMEW0935-9648http://dx.doi.org/10.1002/adma.200900983Google Scholar
K. Goushi et al., “Organic light-emitting diodes employing efficient reverse intersystem crossing for triplet-to-singlet state conversion,” Nat. Photonics 6(4), 253–258 (2012).NPAHBY1749-4885http://dx.doi.org/10.1038/nphoton.2012.31Google Scholar
J. C. Deaton et al., “E-type delayed fluorescence of a phosphine-supported Cu2(mu-NAr2)2 diamond core: harvesting singlet and triplet excitons in OLEDs,” J. Am. Chem. Soc. 132(27), 9499–9508 (2010).JACSAT0002-7863http://dx.doi.org/10.1021/ja1004575Google Scholar
H. Yersin et al., “The triplet state of organo-transition metal compounds. Triplet harvesting and singlet harvesting for efficient OLEDs,” Coord. Chem. Rev. 255(21–22), 2622–2652 (2011).CCHRAM0010-8545http://dx.doi.org/10.1016/j.ccr.2011.01.042Google Scholar
M. Hashimoto et al., “Highly efficient green organic light-emitting diodes containing luminescent three-coordinate copper(I) complexes,” J. Am. Chem. Soc. 133(27), 10348–10351 (2011).JACSAT0002-7863http://dx.doi.org/10.1021/ja202965yGoogle Scholar
A. Tsuboyama et al., “Photophysical properties of highly luminescent copper(I) halide complexes chelated with 1,2-bis(diphenylphosphino)benzene,” Inorg. Chem. 46(6), 1992–2001 (2007).INOCAJ0020-1669http://dx.doi.org/10.1021/ic0608086Google Scholar
D. M. Zink et al., “Synthesis, structure, and characterization of dinuclear copper(I) halide complexes with P^N ligands featuring exciting photoluminescence properties,” Inorg. Chem. 52(5), 2292–2305 (2013).INOCAJ0020-1669http://dx.doi.org/10.1021/ic300979cGoogle Scholar
C. Bizzarri et al., “Luminescent dinuclear Cu(I) complexes containing rigid tetraphosphine ligands,” Inorg. Chem. 53(20), 10944–10951 (2014).INOCAJ0020-1669http://dx.doi.org/10.1021/ic5012204Google Scholar
H. Yersin, R. Czerwieniec, “Organometallic emitters for OLEDs. Triplet harvesting, singlet harvesting, case studies, and trends,” in Physics of Organic Semiconductors, , W. Brütting and C. Adachi, Eds., p. 371, Wiley-VCH, Weinheim, Germany (2012).Google Scholar
M. J. Leitl et al., “Brightly blue and green emitting Cu(I) dimers for singlet harvesting in OLEDs,” J. Phys. Chem. A 117(46), 11823–11836 (2013).JPCAFH1089-5639http://dx.doi.org/10.1021/jp402975dGoogle Scholar
R. Czerwieniec, J. Yu and H. Yersin, “Blue-light emission of Cu(I) complexes and singlet harvesting,” Inorg. Chem. 50(17), 8293–8301 (2011).INOCAJ0020-1669http://dx.doi.org/10.1021/ic200811aGoogle Scholar
D. Volz et al., “High-efficiency OLEDs with fully-bridged PyrPHOS-complexes using singlet harvesting,” Adv. Mater. 27, 2538–2543 (2015).Google Scholar
J. C. Fetzera and M. Zander, “Fluorescence, phosphorescence, and E-type delayed fluorescence of hexabenzo [bc,ef,hi,kl,no,qr] coronene,” Z. Naturforsch. A Phys. Sci. 45(5), 1–3 (1990).http://dx.doi.org/10.1515/zna-1990-0523Google Scholar
Y. Tao et al., “Thermally activated delayed fluorescence materials towards the breakthrough of organoelectronics,” Adv. Mater. 26(47), 7931–7958 (2014).ADVMEW0935-9648http://dx.doi.org/10.1002/adma.v26.47Google Scholar
F. Dumur, “Recent advances in organic light-emitting devices comprising copper complexes: a realistic approach for low-cost and highly emissive devices?” Org. Electron. 21, 27–39 (2015).OERLAU1566-1199http://dx.doi.org/10.1016/j.orgel.2015.02.026Google Scholar
D. Volz et al., “From iridium and platinum to copper and carbon: new avenues for more sustainability in organic light-emitting diodes,” Green Chem. 17(4), 1988–2011 (2015).http://dx.doi.org/10.1039/C4GC02195AGoogle Scholar
P. W. Atkins and R. Friedman, Molecular Quantum Mechanics, 4th ed., Oxford University Press, New York (2005).Google Scholar
J. Shinar, Organic Light-Emitting Devices: A Survey, Springer, New York (2003).Google Scholar
K. Sato et al., “Organic luminescent molecule with energetically equivalent singlet and triplet excited states for organic light-emitting diodes,” Phys. Rev. Lett. 110(24), 247401 (2013).PRLTAO0031-9007http://dx.doi.org/10.1103/PhysRevLett.110.247401Google Scholar
D. Y. Kondakov, “Role of triplet–triplet annihilation in highly efficient fluorescent devices,” J. Soc. Inf. Disp. 17, 137–144 (2009).JSIDE80734-1768http://dx.doi.org/10.1889/JSID17.2.137Google Scholar
Y. Zhang and S. R. Forrest, “Triplet diffusion leads to triplet–triplet annihilation in organic phosphorescent emitters,” Chem. Phys. Lett. 590, 106–110 (2013).CHPLBC0009-2614http://dx.doi.org/10.1016/j.cplett.2013.10.048Google Scholar
D. Y. Kondakov et al., “Triplet annihilation exceeding spin statistical limit in highly efficient fluorescent organic light-emitting diodes,” J. Appl. Phys. 106(12), 124510 (2009).JAPIAU0021-8979http://dx.doi.org/10.1063/1.3273407Google Scholar
P.-Y. Chou et al., “Efficient delayed fluorescence via triplet–triplet annihilation for deep-blue electroluminescence,” Chem. Commun. 50(52), 6869 (2014).http://dx.doi.org/10.1039/c4cc01851fGoogle Scholar
Y. Seino et al., “High-performance blue phosphorescent OLEDs using energy transfer from exciplex,” Adv. Mater. 26(10), 1612–1616 (2014).ADVMEW0935-9648http://dx.doi.org/10.1002/adma.201304253Google Scholar
J.-H. Lee et al., “An exciplex forming host for highly efficient blue organic light emitting diodes with low driving voltage,” Adv. Funct. Mater. 25(3), 361–366 (2014).AFMDC61616-301Xhttp://dx.doi.org/10.1002/adfm.201402707Google Scholar
Y.-S. Park, K.-H. Kim and J.-J. Kim, “Efficient triplet harvesting by fluorescent molecules through exciplexes for high efficiency organic light-emitting diodes,” Appl. Phys. Lett. 102, 153306 (2013).APPLAB0003-6951http://dx.doi.org/10.1063/1.4802716Google Scholar
Y.-S. Park et al., “Exciplex-forming co-host for organic light-emitting diodes with ultimate efficiency,” Adv. Funct. Mater. 23(39), 4914–4920 (2013).AFMDC61616-301Xhttp://dx.doi.org/10.1002/adfm.v23.39Google Scholar
M. Montalti et al., Handbook of Photochemistry, CRC Press, Boca Raton (2006).Google Scholar
N. J. Turro, Modern Molecular Photochemistry, University Science Books, Sausalito (1991).Google Scholar
C. Y. Kwong et al., “Efficiency and stability of different tris(8-hydroxyquinoline) aluminium (Alq3) derivatives in OLED applications,” Mater. Sci. Eng. B 116(1), 75–81 (2005).MSBTEK0921-5107http://dx.doi.org/10.1016/j.mseb.2004.09.024Google Scholar
F. P. Rosselli et al., “Experimental and theoretical investigation of tris-(8-hydroxy-quinolinate) aluminum (Alq3) photo degradation,” Org. Electron. 10(8), 1417–1423 (2009).OERLAU1566-1199http://dx.doi.org/10.1016/j.orgel.2009.08.026Google Scholar
H. D. Burrows et al., “Characterization of the triplet state of tris(8-hydroxyquinoline)aluminium(III) in benzene solution,” J. Am. Chem. Soc. 125(50), 15310–15311 (2003).JACSAT0002-7863http://dx.doi.org/10.1021/ja037254fGoogle Scholar
B. Minaev, G. Baryshnikov and H. Agren, “Principles of phosphorescent organic light emitting devices,” Phys. Chem. Chem. Phys. 16(5), 1719–1758 (2014).PPCPFQ1463-9076http://dx.doi.org/10.1039/C3CP53806KGoogle Scholar
M. A. Baldo et al., “Very high-efficiency green organic light-emitting devices based on electrophosphorescence,” Appl. Phys. Lett. 75(1), 4 (1999).APPLAB0003-6951http://dx.doi.org/10.1063/1.124258Google Scholar
J. C. Ribierre et al., “Temperature dependence of the triplet diffusion and quenching rates in films of an Irppy3-cored dendrimer,” Phys. Rev. B: Condens. Matter 77(8), 085211 (2008).http://dx.doi.org/10.1103/PhysRevB.77.085211Google Scholar
S. Takayasu, T. Suzuki and K. Shinozaki, “Intermolecular interactions and aggregation of fac-tris(2-phenylpyridinato-C2, N)iridium(III) in nonpolar solvents,” J. Phys. Chem. B 117(32), 9449–9456 (2013).JPCBFK1520-6106http://dx.doi.org/10.1021/jp403974hGoogle Scholar
H. Yersin, R. Czerwieniec and A. Hupfer, “Singlet harvesting with brightly emitting Cu(I) and metal-free organic compounds,” Proc. SPIE 8435, 843508 (2012).PSISDG0277-786Xhttp://dx.doi.org/10.1117/12.921372Google Scholar
R. Ishimatsu et al., “Solvent effect on thermally activated delayed fluorescence by 1,2,3,5-tetrakis(carbazol-9-yl)-4,6-dicyanobenzene,” J. Phys. Chem. A 117(27), 5607–5612 (2013).JPCAFH1089-5639http://dx.doi.org/10.1021/jp404120sGoogle Scholar
Y. Im and J. Y. Lee, “Above 20% external quantum efficiency in thermally activated delayed fluorescence device using furodipyridine-type host materials,” Chem. Mater. 26(3), 1413–1419 (2014).CMATEX0897-4756http://dx.doi.org/10.1021/cm403358hGoogle Scholar
O. Y. Kim, B. S. Kim and J. Y. Lee, “High efficiency thermally activated delayed fluorescent devices using a mixed host of carbazole and phosphine oxide derived host materials,” Synth. Met. 201, 49–53 (2015).SYMEDZ0379-6779http://dx.doi.org/10.1016/j.synthmet.2014.12.025Google Scholar
M. Leung et al., “Novel ambipolar orthogonal donor–acceptor host for blue organic light emitting diodes,” Org. Lett. 15(18), 4694–4697 (2013).ORLEF71523-7060http://dx.doi.org/10.1021/ol402001vGoogle Scholar
D. Kim, L. Zhu and J.-L. Brédas, “Electronic structure of carbazole-based phosphine oxides as ambipolar host materials for deep blue electrophosphorescence: a density functional theory study,” Chem. Mater. 24(13), 2604–2610 (2012).CMATEX0897-4756http://dx.doi.org/10.1021/cm301416nGoogle Scholar
M. S. Park and J. Y. Lee, “9-(Pyridin-3-yl)-9H-carbazole derivatives as host materials for green phosphorescent organic light-emitting diodes,” Org. Electron. 14(5), 1291–1296 (2013).OERLAU1566-1199http://dx.doi.org/10.1016/j.orgel.2013.02.036Google Scholar
H.-F. Chen et al., “1,3,5-Triazine derivatives as new electron transport-type host materials for highly efficient green phosphorescent OLEDs,” J. Mater. Chem. 19, 8112 (2009).JMACEP0959-9428http://dx.doi.org/10.1039/b913423aGoogle Scholar
Y. Seino et al., “Novel blue exciplex comprising acridine and sulfone derivatives as a host material for high-efficiency blue phosphorescent OLEDs,” Chem. Lett. 45(3), 283–285 (2016).CMLTAG0366-7022http://dx.doi.org/10.1246/cl.151094Google Scholar
C. Tang et al., “A versatile efficient one-step approach for carbazole–pyridine hybrid molecules: highly efficient host materials for blue phosphorescent OLEDs,” Chem. Commun. 51, 1650–1653 (2014).http://dx.doi.org/10.1039/C4CC08335KGoogle Scholar
H. Tanaka et al., “Efficient green thermally activated delayed fluorescence (TADF) from a phenoxazine–triphenyltriazine (PXZ–TRZ) derivative,” Chem. Commun. 48(93), 11392–11394 (2012).http://dx.doi.org/10.1039/c2cc36237fGoogle Scholar
D. Zhang et al., “Highly efficient blue thermally activated delayed fluorescent OLEDs with record-low driving voltages utilizing high triplet energy hosts with small singlet–triplet splittings,” Chem. Sci. 25, 1–9 (2016).1478-6524http://dx.doi.org/10.1039/C5SC04755BGoogle Scholar
F. B. Dias et al., “Triplet harvesting with 100% efficiency by way of thermally activated delayed fluorescence in charge transfer OLED emitters,” Adv. Mater. 25(27), 3707–3714 (2013).ADVMEW0935-9648http://dx.doi.org/10.1002/adma.v25.27Google Scholar
M. Kim et al., “Highly efficient and color tunable thermally activated delayed fluorescent emitters using a ‘twin emitter’ molecular design,” Chem. Commun. 52, 339–342 (2015).http://dx.doi.org/10.1039/C5CC07999CGoogle Scholar
J. Li et al., “Highly efficient organic light-emitting diode based on a hidden thermally activated delayed fluorescence channel in a heptazine derivative,” Adv. Mater. 25(24), 3319–3323 (2013).ADVMEW0935-9648http://dx.doi.org/10.1002/adma.v25.24Google Scholar
Y. Sagara et al., “Highly efficient thermally activated delayed fluorescence emitters with a small singlet–triplet energy gap and large oscillator strength,” Chem. Lett. 44(3), 360–362 (2015).CMLTAG0366-7022http://dx.doi.org/10.1246/cl.141054Google Scholar
A. Endo et al., “Efficient up-conversion of triplet excitons into a singlet state and its application for organic light emitting diodes,” Appl. Phys. Lett. 98(8), 083302 (2011).APPLAB0003-6951http://dx.doi.org/10.1063/1.3558906Google Scholar
W. Liu et al., “Novel carbazol–pyridine–carbonitrile derivative as excellent blue thermally activated delayed fluorescence emitter for highly efficient organic light-emitting devices,” ACS Appl. Mater. Interfaces 7(34), 18930–18936 (2015).AAMICK1944-8244http://dx.doi.org/10.1021/acsami.5b05648Google Scholar
K. Masui, H. Nakanotani and C. Adachi, “Analysis of exciton annihilation in high-efficiency sky-blue organic light-emitting diodes with thermally activated delayed fluorescence,” Org. Electron. 14(11), 2721–2726 (2013).http://dx.doi.org/10.1016/j.orgel.2013.07.010Google Scholar
D. R. Lee et al., “Above 30% external quantum efficiency in green delayed fluorescent organic light-emitting diodes,” ACS Appl. Mater. Interfaces 7(18), 9625–9629 (2015).AAMICK1944-8244http://dx.doi.org/10.1021/acsami.5b01220Google Scholar
Y. Li et al., “Deep blue fluorophores incorporating sulfone-locked triphenylamine: the key for highly efficient fluorescence–phosphorescence hybrid white OLEDs with simplified structure,” J. Mater. Chem. C 3, 6986–6996 (2015).http://dx.doi.org/10.1039/C5TC01373AGoogle Scholar
Q. Zhang et al., “Design of efficient thermally activated delayed fluorescence materials for pure blue organic light emitting diodes,” J. Am. Chem. Soc. 134(36), 14706–14709 (2012).JACSAT0002-7863http://dx.doi.org/10.1021/ja306538wGoogle Scholar
D. R. Lee et al., “Design strategy for 25% external quantum efficiency in green and blue thermally activated delayed fluorescent devices,” Adv. Mater. 27(39), 5861–5867 (2015).ADVMEW0935-9648http://dx.doi.org/10.1002/adma.201502053Google Scholar
M. Kim et al., “Stable blue thermally activated delayed fluorescent organic light-emitting diodes with three times longer lifetime than phosphorescent organic light-emitting diodes,” Adv. Mater. 27(15), 2515–2520 (2015).ADVMEW0935-9648http://dx.doi.org/10.1002/adma.201500267Google Scholar
Y. Tao et al., “Tuning the optoelectronic properties of carbazole/oxadiazole hybrids through linkage modes: hosts for highly efficient green electrophosphorescence,” Adv. Funct. Mater. 20, 304–311 (2010).AFMDC61616-301Xhttp://dx.doi.org/10.1002/adfm.v20:2Google Scholar
J. Lee et al., “Oxadiazole- and triazole-based highly-efficient thermally activated delayed fluorescence emitters for organic light-emitting diodes,” J. Mater. Chem. C 1(30), 4599 (2013).http://dx.doi.org/10.1039/c3tc30699bGoogle Scholar
A. E. Nikolaenko et al., “Thermally activated delayed fluorescence in polymers: a new route toward highly efficient solution processable OLEDs,” Adv. Mater. 27(44), 7236–7240 (2015).ADVMEW0935-9648http://dx.doi.org/10.1002/adma.201501090Google Scholar
Y. Sakai et al., “Zinc complexes exhibiting highly efficient thermally activated delayed fluorescence and their application to organic light-emitting diodes,” Chem. Commun. 51(15), 3181–3184 (2015).http://dx.doi.org/10.1039/C4CC09403DGoogle Scholar
D. Volz et al., “Bridging the efficiency gap: fully bridged dinuclear Cu(I)-complexes for singlet harvesting in high-efficiency OLEDs,” Adv. Mater. 27(15), 2538–2543 (2015).ADVMEW0935-9648http://dx.doi.org/10.1002/adma.201405897Google Scholar
J. W. Sun et al., “A fluorescent organic light-emitting diode with 30% external quantum efficiency,” Adv. Mater. 26(32), 5684–5688 (2014).ADVMEW0935-9648http://dx.doi.org/10.1002/adma.201401407Google Scholar
S.-Y. Y. Kim et al., “Organic light-emitting diodes with 30% external quantum efficiency based on a horizontally oriented emitter,” Adv. Funct. Mater. 23(31), 3896–3900 (2013).AFMDC61616-301Xhttp://dx.doi.org/10.1002/adfm.v23.31Google Scholar
M. Wallesch et al., “Bright coppertunities: multinuclear CuI complexes with N–P ligands and their applications,” Chem. Eur. J. 20(22), 6578–6590 (2014).http://dx.doi.org/10.1002/chem.201402060Google Scholar
M. Wallesch et al., “Bright coppertunities: efficient OLED devices with copper(I)iodide-NHetPHOS-emitters,” Proc. SPIE 9183, 918309 (2014).PSISDG0277-786Xhttp://dx.doi.org/10.1117/12.2060499Google Scholar
D. M Zink et al., “Novel oligonuclear copper complexes featuring exciting luminescent characteristics,” Proc. SPIE 8829, 882907 (2013).PSISDG0277-786Xhttp://dx.doi.org/10.1117/12.2028619Google Scholar
H. Nakanotani et al., “Promising operational stability of high-efficiency organic light-emitting diodes based on thermally activated delayed fluorescence,” Sci. Rep. 3, 2127 (2013).SRCEC32045-2322http://dx.doi.org/10.1038/srep02127Google Scholar
Q. Zhang et al., “Triplet exciton confinement in green organic light-emitting diodes containing luminescent charge-transfer Cu(I) complexes,” Adv. Funct. Mater. 22(11), 2327–2336 (2012).AFMDC61616-301Xhttp://dx.doi.org/10.1002/adfm.v22.11Google Scholar
Y. Noguchi et al., “Charge carrier dynamics and degradation phenomena in organic light-emitting diodes doped by a thermally activated delayed fluorescence emitter,” Org. Electron. 17, 184–191 (2014).OERLAU1566-1199http://dx.doi.org/10.1016/j.orgel.2014.12.009Google Scholar
F. So and D. Kondakov, “Degradation mechanisms in small-molecule and polymer organic light-emitting diodes,” Adv. Mater. 22(34), 3762–3777 (2010).ADVMEW0935-9648http://dx.doi.org/10.1002/adma.200902624Google Scholar
A. S. D. Sandanayaka, T. Matsushima and C. Adachi, “Degradation mechanisms of organic light-emitting diodes based on thermally activated delayed fluorescence molecules,” J. Phys. Chem. C 119(42), 23845–23851 (2015).JPCCCK1932-7447http://dx.doi.org/10.1021/acs.jpcc.5b07084Google Scholar
S. Wang et al., “Achieving high power efficiency and low roll-off OLEDs based on energy transfer from thermally activated delayed excitons to fluorescent dopants,” Chem. Commun. 51, 11972–11975 (2015).http://dx.doi.org/10.1039/C5CC04469CGoogle Scholar
T. Komino et al., “Suppression of efficiency roll-off characteristics in thermally activated delayed fluorescence based organic light-emitting diodes using randomly oriented host molecules,” Chem. Mater. 25(15), 3038–3047 (2013).CMATEX0897-4756http://dx.doi.org/10.1021/cm4011597Google Scholar
S. Wu et al., “High-efficiency deep-blue organic light-emitting diodes based on a thermally activated delayed fluorescence emitter,” J. Mater. Chem. C 2(3), 421–424 (2014).http://dx.doi.org/10.1039/C3TC31936AGoogle Scholar
M. Zhu and C. Yang, “Blue fluorescent emitters: design tactics and applications in organic light-emitting diodes,” Chem. Soc. Rev. 42(12), 4963–4976 (2013).CSRVBR0306-0012http://dx.doi.org/10.1039/c3cs35440gGoogle Scholar
Y. Zhang, J. Lee and S. R. Forrest, “Tenfold increase in the lifetime of blue phosphorescent organic light-emitting diodes,” Nat. Commun. 5, 1–7 (2014).NCAOBW2041-1723http://dx.doi.org/10.1038/ncomms6008Google Scholar
R. Seifert et al., “Chemical degradation mechanisms of highly efficient blue phosphorescent emitters used for organic light emitting diodes,” Org. Electron. 14(1), 115–123 (2013).OERLAU1566-1199http://dx.doi.org/10.1016/j.orgel.2012.10.003Google Scholar
S. Schmidbauer, A. Hohenleutner and B. König, “Studies on the photodegradation of red, green and blue phosphorescent OLED emitters,” Beilstein J.Org. Chem. 9, 2088–2096 (2013).http://dx.doi.org/10.3762/bjoc.9.245Google Scholar
R. Seifert et al., “Comparison of ultraviolet- and charge-induced degradation phenomena in blue fluorescent organic light emitting diodes,” Appl. Phys. Lett. 97(1), 013308 (2010).APPLAB0003-6951http://dx.doi.org/10.1063/1.3460285Google Scholar
Q. Wang and H. Aziz, “Degradation of organic/organic interfaces in organic light-emitting devices due to polaron–exciton interactions,” ACS Appl. Mater. Interfaces 5(17), 8733–8739 (2013).AAMICK1944-8244http://dx.doi.org/10.1021/am402537jGoogle Scholar
Y. Luo et al., “Similar roles of electrons and holes in luminescence degradation of organic light-emitting devices,” Chem. Mater. 19(8), 2079–2083 (2007).CMATEX0897-4756http://dx.doi.org/10.1021/cm062621iGoogle Scholar
T. D. Schmidt et al., “Degradation induced decrease of the radiative quantum efficiency in organic light-emitting diodes,” Appl. Phys. Lett. 101(10), 103301 (2012).APPLAB0003-6951http://dx.doi.org/10.1063/1.4749815Google Scholar
I. Lee and J. Y. Lee, “Molecular design of deep blue fluorescent emitters with 20% external quantum efficiency and narrow emission spectrum,” Org. Electron. 29, 160–164 (2016).http://dx.doi.org/10.1016/j.orgel.2015.12.001Google Scholar
Daniel Volz studied chemistry at the KIT and the KSOP in Karlsruhe, Germany, in the group of Professor Stefan Bräse and received his PhD in 2014. He is a team leader and one of the leading scientists at the CYNORA GmbH. He joined CYNORA’s R&D Division in 2009. Since 2015, he has been involved in the company’s R&D strategy. His research interests are aimed toward the development of new, sustainable emitting materials for OLEDs, and exploration of their photophysical and processing properties.